2. Mechanics of Materials: Strain. 3. Hookes's Law


 Buck Hensley
 2 years ago
 Views:
Transcription
1 Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate Transformations 3. Principal Stress for the Case of Plane Stress 4. Mohr's Circle for Plane Stress 5. Mohr's Circle Usage in Plane Stress 6. Examples of Mohr's Circles in Plane Stress 2. Mechanics of Materials: Strain 1. Introduction 2. Plane Strain and Coordinate Transformations 3. Principal Strain for the Case of Plane Strain 4. Mohr's Circle for Plane Strain 5. Mohr's Circle Usage in Plane Strain 6. Examples of Mohr's Circles in Plane Strain 3. Hookes's Law 1. Introduction 2. Orthotropic Material 3. Transverse Isotropic 4. Isotropic Material 5. Plane Stress 6. Plane Strain Finding E and ν 8. Finding G and K Failure Criteria 1. Introduction 2. Yield of Ductile Material 3. Failure of Brittle Material 4. Prevention/Diagnosis Back to top Last modified Tuesday December 11, 2001 by: Sape A. Miedema Copyright December, 2001 Dr.ir. S.A. Miedema (1 of 2) [12/13/ :59:54]
2 Mechanics of Materials Download Adobe Acrobat Reader V4.0 (2 of 2) [12/13/ :59:54]
3 Mechanics of Materials: Stress Mechanics of Materials: Stress The Definition of Stress The concept of stress originated from the study of strength and failure of solids. The stress field is the distribution of internal "tractions" that balance a given set of external tractions and body forces. First, we look at the external traction T that represents the force per unit area acting at a given location on the body's surface. Traction T is a bound vector, which means T cannot slide along its line of action or translate to another location and keep the same meaning. In other words, a traction vector cannot be fully described unless both the force and the surface where the force acts on has been specified. Given both F and s, the traction T can be defined as The internal traction within a solid, or stress, can be defined in a similar manner. Suppose an arbitrary slice is made across the solid shown in the above figure, leading to the free body diagram shown at right. Surface tractions would appear on the exposed surface, similar in form to the external tractions applied to the body's exterior surface. The stress at point P can be defined using the same equation as was used for T. Stress therefore can be interpreted as internal tractions that act on a defined internal datum plane. One cannot measure the stress without first specifying the datum plane. The Stress Tensor (or Stress Matrix) (1 of 3) [12/13/ :59:57]
4 Mechanics of Materials: Stress Surface tractions, or stresses acting on an internal datum plane, are typically decomposed into three mutually orthogonal components. One component is normal to the surface and represents direct stress. The other two components are tangential to the surface and represent shear stresses. What is the distinction between normal and tangential tractions, or equivalently, direct and shear stresses? Direct stresses tend to change the volume of the material (e.g. hydrostatic pressure) and are resisted by the body's bulk modulus (which depends on the Young's modulus and Poisson ratio). Shear stresses tend to deform the material without changing its volume, and are resisted by the body's shear modulus. Defining a set of internal datum planes aligned with a Cartesian coordinate system allows the stress state at an internal point P to be described relative to x, y, and z coordinate directions. For example, the stress state at point P can be represented by an infinitesimal cube with three stress components on each of its six sides (one direct and two shear components). Since each point in the body is under static equilibrium (no net force in the absense of any body forces), only nine stress components from three planes are needed to describe the stress state at a point P. These nine components can be organized into the matrix: where shear stresses across the diagonal are identical (i.e. σ xy = σ yx, σ yz = σ zy, and σ zx = σ xz ) as a result of static equilibrium (no net moment). This grouping of the nine stress components is known as the stress tensor (or stress matrix). The subscript notation used for the nine stress components have the following meaning: (2 of 3) [12/13/ :59:57]
5 Mechanics of Materials: Stress Note: The stress state is a second order tensor since it is a quantity associated with two directions. As a result, stress components have 2 subscripts. A surface traction is a first order tensor (i.e. vector) since it a quantity associated with only one direction. Vector components therefore require only 1 subscript. Mass would be an example of a zeroorder tensor (i.e. scalars), which have no relationships with directions (and no subscripts). Equations of Equilibrium Consider the static equilibrium of a solid subjected to the body force vector field b. Applying Newton's first law of motion results in the following set of differential equations which govern the stress distribution within the solid, In the case of two dimensional stress, the above equations reduce to, (3 of 3) [12/13/ :59:57]
6 Plane Stress and Coordinate Transformations Plane Stress and Coordinate Transformations Plane State of Stress A class of common engineering problems involving stresses in a thin plate or on the free surface of a structural element, such as the surfaces of thinwalled pressure vessels under external or internal pressure, the free surfaces of shafts in torsion and beams under transverse load, have one principal stress that is much smaller than the other two. By assuming that this small principal stress is zero, the threedimensional stress state can be reduced to two dimensions. Since the remaining two principal stresses lie in a plane, these simplified 2D problems are called plane stress problems. Assume that the negligible principal stress is oriented in the zdirection. To reduce the 3D stress matrix to the 2D plane stress matrix, remove all components with z subscripts to get, where τ xy = τ yx for static equilibrium. The sign convention for positive stress components in plane stress is illustrated in the above figure on the 2D element. Coordinate Transformations The coordinate directions chosen to analyze a structure are usually based on the shape of the structure. As a result, the direct and shear stress components are associated with these directions. For example, to analyze a bar one almost always directs one of the coordinate directions along the bar's axis. Nonetheless, stresses in directions that do not line up with the original coordinate set are also important. For example, the failure plane of a brittle shaft under torsion is often at a 45 angle with respect to the shaft's axis. Stress transformation formulas are required to analyze these stresses. The transformation of stresses with respect to the {x,y,z} coordinates to the stresses with respect to {x',y',z'} is performed via the equations, (1 of 2) [12/13/ :59:58]
7 Plane Stress and Coordinate Transformations where θ is the rotation angle between the two coordinate sets (positive in the counterclockwise direction). This angle along with the stresses for the {x',y',z'} coordinates are shown in the figure below, (2 of 2) [12/13/ :59:58]
8 Principal Stress for the Case of Plane Stress Principal Stress for the Case of Plane Stress Principal Directions, Principal Stress The normal stresses (σ x' and σ y' ) and the shear stress (τ x'y' ) vary smoothly with respect to the rotation angle θ, in accordance with the coordinate transformation equations. There exist a couple of particular angles where the stresses take on special values. First, there exists an angle θ p where the shear stress τ x'y' becomes zero. That angle is found by setting τ x'y' to zero in the above shear transformation equation and solving for θ (set equal to θ p ). The result is, The angle θ p defines the principal directions where the only stresses are normal stresses. These stresses are called principal stresses and are found from the original stresses (expressed in the x,y,z directions) via, The transformation to the principal directions can be illustrated as: (1 of 2) [12/13/ :59:59]
9 Principal Stress for the Case of Plane Stress Maximum Shear Stress Direction Another important angle, θ s, is where the maximum shear stress occurs. This is found by finding the maximum of the shear stress transformation equation, and solving for θ. The result is, The maximum shear stress is equal to onehalf the difference between the two principal stresses, The transformation to the maximum shear stress direction can be illustrated as: (2 of 2) [12/13/ :59:59]
10 Mohr's Circle for Plane Stress Mohr's Circle for Plane Stress Mohr's Circle Introduced by Otto Mohr in 1882, Mohr's Circle illustrates principal stresses and stress transformations via a graphical format, The two principal stresses are shown in red, and the maximum shear stress is shown in orange. Recall that the normal stesses equal the principal stresses when the stress element is aligned with the principal directions, and the shear stress equals the maximum shear stress when the stress element is rotated 45 away from the principal directions. As the stress element is rotated away from the principal (or maximum shear) directions, the normal and shear stress components will always lie on Mohr's Circle. Mohr's Circle was the leading tool used to visualize relationships between normal and shear stresses, and to estimate the maximum stresses, before handheld calculators became popular. Even today, Mohr's Circle is still widely used by engineers all over the world. Derivation of Mohr's Circle To establish Mohr's Circle, we first recall the stress transformation formulas for plane stress at a given location, Using a basic trigonometric relation (cos 2 2θ + sin 2 2θ = 1) to combine the two above equations we have, (1 of 2) [12/13/ :00:01]
11 Mohr's Circle for Plane Stress This is the equation of a circle, plotted on a graph where the abscissa is the normal stress and the ordinate is the shear stress. This is easier to see if we interpret σ x and σ y as being the two principal stresses, and τ xy as being the maximum shear stress. Then we can define the average stress, σ avg, and a "radius" R (which is just equal to the maximum shear stress), The circle equation above now takes on a more familiar form, The circle is centered at the average stress value, and has a radius R equal to the maximum shear stress, as shown in the figure below, Related Topics The procedure of drawing a Mohr's Circle from a given stress state is discussed in the Mohr's Circle usage page. The Mohr's Circle for plane strain can also be obtained from similar procedures. (2 of 2) [12/13/ :00:01]
12 Mohr's Circle Usage in Plane Stress Mohr's Circle Usage in Plane Stress Principal Stresses from Mohr's Circle A chief benefit of Mohr's circle is that the principal stresses σ 1 and σ 2 and the maximum shear stress τ max are obtained immediately after drawing the circle, where, Principal Directions from Mohr's Circle Mohr's Circle can be used to find the directions of the principal axes. To show this, first suppose that the normal and shear stresses, σ x, σ y, and τ xy, are obtained at a given point O in the body. They are expressed relative to the coordinates XY, as shown in the stress element at right below. The Mohr's Circle for this general stress state is shown at left above. Note that it's centered at σ avg and has a radius R, and that the two points {σ x, τ xy } and {σ y, τ xy } lie on opposites sides of the circle. The line connecting σ x and σ y will be defined as L xy. The angle between the current axes (X and Y) and the principal axes is defined as θ p, and is equal to one half the angle between the line L xy and the σaxis as shown in the schematic below, (1 of 4) [12/13/ :00:03]
13 Mohr's Circle Usage in Plane Stress A set of six Mohr's Circles representing most stress state possibilities are presented on the examples page. Also, principal directions can be computed by the principal stress calculator. Rotation Angle on Mohr's Circle Note that the coordinate rotation angle θ p is defined positive when starting at the XY coordinates and proceeding to the X p Y p coordinates. In contrast, on the Mohr's Circle θ p is defined positive starting on the principal stress line (i.e. the σaxis) and proceeding to the XY stress line (i.e. line L xy ). The angle θ p has the opposite sense between the two figures, because on one it starts on the XY coordinates, and on the other it starts on the principal coordinates. Some books avoid this dichotomy between θ p on Mohr's Circle and θ p on the stress element by locating (σ x, τ xy ) instead of (σ x, τ xy ) on Mohr's Circle. This will switch the polarity of θ p on the circle. Whatever method you choose, the bottom line is that an opposite sign is needed either in the interpretation or in the plotting to make Mohr's Circle physically meaningful. Stress Transform by Mohr's Circle (2 of 4) [12/13/ :00:03]
14 Mohr's Circle Usage in Plane Stress Mohr's Circle can be used to transform stresses from one coordinate set to another, similar that that described on the plane stress page. Suppose that the normal and shear stresses, σ x, σ y, and τ xy, are obtained at a point O in the body, expressed with respect to the coordinates XY. We wish to find the stresses expressed in the new coordinate set X'Y', rotated an angle θ from XY, as shown below: To do this we proceed as follows: Draw Mohr's circle for the given stress state (σ x, σ y, and τ xy ; shown below). Draw the line L xy across the circle from (σ x, τ xy ) to (σ y, τ xy ). Rotate the line L xy by 2*θ (twice as much as the angle between XY and X'Y') and in the opposite direction of θ. The stresses in the new coordinates (σ x', σ y', and τ x'y' ) are then read off the circle. (3 of 4) [12/13/ :00:03]
15 Mohr's Circle Usage in Plane Stress Stress transforms can be performed using efunda's stress transform calculator. (4 of 4) [12/13/ :00:03]
16 Examples of Mohr's Circles in Plane Stress Examples of Mohr's Circles in Plane Stress Case 1: τ xy > 0 and σ x > σ y The principal axes are counterclockwise to the current axes (because τ xy > 0) and no more than 45º away (because σ x > σ y ). Case 2: τ xy < 0 and σ x > σ y The principal axes are clockwise to the current axes (because τ xy < 0) and no more than 45º away (because σ x > σ y ). Case 3: τ xy > 0 and σ x < σ y (1 of 3) [12/13/ :00:05]
17 Examples of Mohr's Circles in Plane Stress The principal axes are counterclockwise to the current axes (because τ xy > 0) and between 45º and 90º away (because σ x < σ y ). Case 4: τ xy < 0 and σ x < σ y The principal axes are clockwise to the current axes (because τ xy < 0) and between 45º and 90º away (because σ x < σ y ). Case 5: τ xy = 0 and σ x > σ y (2 of 3) [12/13/ :00:05]
18 Examples of Mohr's Circles in Plane Stress The principal axes are aligned with the current axes (because σ x > σ y and τ xy = 0). Case 6: τ xy = 0 and σ x < σ y The principal axes are exactly 90 from the current axes (because σ x < σ y and τ xy = 0). (3 of 3) [12/13/ :00:05]
19 Mechanics of Materials: Strain Mechanics of Materials: Strain Global 1D Strain Consider a rod with initial length L which is stretched to a length L'. The strain measure ε, a dimensionless ratio, is defined as the ratio of elongation with respect to the original length, Infinitesimal 1D Strain The above strain measure is defined in a global sense. The strain at each point may vary dramatically if the bar's elastic modulus or crosssectional area changes. To track down the strain at each point, further refinement in the definition is needed. Consider an arbitrary point in the bar P, which has a position vector x, and its infinitesimal neighbor dx. Point P shifts to P', which has a position vector x', after the stretch. In the meantime, the small "step" dx is stretched to dx'. The strain at point p can be defined the same as in the global strain measure, hence be rewritten as, Since the displacement, the strain can General Definition of 3D Strain (1 of 4) [12/13/ :00:07]
20 Mechanics of Materials: Strain As in the one dimensional strain derivation, suppose that point P in a body shifts to point P after deformation. The infinitesimal straindisplacement relationships can be summarized as, where u is the displacement vector, x is coordinate, and the two indices i and j can range over the three coordinates {1, 2, 3} in three dimensional space. Expanding the above equation for each coordinate direction gives, where u, v, and w are the displacements in the x, y, and z directions respectively (i.e. they are the (2 of 4) [12/13/ :00:07]
21 Mechanics of Materials: Strain components of u). 3D Strain Matrix There are a total of 6 strain measures. These 6 measures can be organized into a matrix (similar in form to the 3D stress matrix), shown here, Engineering Shear Strain Focus on the strain ε xy for a moment. The expression inside the parentheses can be rewritten as, where. Called the engineering shear strain, γ xy is a total measure of shear strain in the xy plane. In contrast, the shear strain ε xy is the average of the shear strain on the x face along the y direction, and on the y face along the x direction. Engineering shear strain is commonly used in engineering reference books. However, please beware of the difference between shear strain and engineering shear strain, so as to avoid errors in mathematical manipulations. Compatibility Conditions (3 of 4) [12/13/ :00:07]
22 Mechanics of Materials: Strain In the straindisplacement relationships, there are six strain measures but only three independent displacements. That is, there are 6 unknowns for only 3 independent variables. As a result there exist 3 constraint, or compatibility, equations. These compatibility conditions for infinitesimal strain reffered to rectangular Cartesian coordinates are, In two dimensional problems (e.g. plane strain), all z terms are set to zero. The compatibility equations reduce to, Note that some references use engineering shear strain ( compatibility equations. ) when referencing (4 of 4) [12/13/ :00:07]
23 Plane Strain and Coordinate Transformations Plane Strain and Coordinate Transformations Plane State of Strain Some common engineering problems such as a dam subjected to water loading, a tunnel under external pressure, a pipe under internal pressure, and a cylindrical roller bearing compressed by force in a diametral plane, have significant strain only in a plane; that is, the strain in one direction is much less than the strain in the two other orthogonal directions. If small enough, the smallest strain can be ignored and the part is said to experience plane strain. Assume that the negligible strain is oriented in the zdirection. To reduce the 3D strain matrix to the 2D plane stress matrix, remove all components with z subscripts to get, where ε xy = ε yx by definition. The sign convention here is consistent with the sign convention used in plane stress analysis. Coordinate Transformation The transformation of strains with respect to the {x,y,z} coordinates to the strains with respect to {x',y',z'} is performed via the equations, The rotation between the two coordinate sets is shown here, (1 of 2) [12/13/ :00:08]
24 Plane Strain and Coordinate Transformations where θ is defined positive in the counterclockwise direction. (2 of 2) [12/13/ :00:08]
25 Principal Strain for the Case of Plane Strain Principal Strain for the Case of Plane Strain Principal Directions, Principal Strain The normal strains (ε x' and ε y' ) and the shear strain (ε x'y' ) vary smoothly with respect to the rotation angle θ, in accordance with the transformation equations given above. There exist a couple of particular angles where the strains take on special values. First, there exists an angle θ p where the shear strain ε x'y' vanishes. That angle is given by, This angle defines the principal directions. The associated principal strains are given by, The transformation to the principal directions with their principal strains can be illustrated as: Maximum Shear Strain Direction (1 of 2) [12/13/ :00:09]
26 Principal Strain for the Case of Plane Strain Another important angle, θ s, is where the maximum shear strain occurs and is given by, The maximum shear strain is found to be onehalf the difference between the two principal strains, The transformation to the maximum shear strain direction can be illustrated as: (2 of 2) [12/13/ :00:09]
27 Mohr's Circle for Plane Strain Mohr's Circle for Plane Strain Mohr's Circle Strains at a point in the body can be illustrated by Mohr's Circle. The idea and procedures are exactly the same as for Mohr's Circle for plane stress. The two principal strains are shown in red, and the maximum shear strain is shown in orange. Recall that the normal strains are equal to the principal strains when the element is aligned with the principal directions, and the shear strain is equal to the maximum shear strain when the element is rotated 45 away from the principal directions. As the element is rotated away from the principal (or maximum strain) directions, the normal and shear strain components will always lie on Mohr's Circle. Derivation of Mohr's Circle To establish the Mohr's circle, we first recall the strain transformation formulas for plane strain, Using a basic trigonometric relation (cos 2 2θ + sin 2 2θ = 1) to combine the above two formulas we have, This equation is an equation for a circle. To make this more apparent, we can rewrite it as, (1 of 2) [12/13/ :00:11]
28 Mohr's Circle for Plane Strain where, The circle is centered at the average strain value ε Avg, and has a radius R equal to the maximum shear strain, as shown in the figure below, Related Topics The procedure of drawing Mohr's Circle from a given strain state is discussed in the Mohr's Circle usage and examples pages. The Mohr's Circle for plane stress can also be obtained from similar procedures. (2 of 2) [12/13/ :00:11]
29 Mohr's Circle Usage in Plane Strain Mohr's Circle Usage in Plane Strain Principal Strains from Mohr's Circle A chief benefit of Mohr's circle is that the principal strains ε 1 and ε 2 and the maximum shear strain ε xymax are obtained immediately after drawing the circle, where, Principal Directions from Mohr's Circle Mohr's Circle can be used to find the directions of the principal axes. To show this, first suppose that the normal and shear strains, ε x, ε y, and ε xy, are obtained at a given point O in the body. They are expressed relative to the coordinates XY, as shown in the strain element at right below. The Mohr's Circle for this general strain state is shown at left above. Note that it's centered at ε Avg and has a radius R, and that the two points (ε x, ε xy ) and (ε y, ε xy ) lie on opposites sides of the circle. The line connecting ε x and ε y will be defined as L xy. The angle between the current axes (X and Y) and the principal axes is defined as θ p, and is equal to one half the angle between the line L xy and the εaxis as shown in the schematic below, (1 of 4) [12/13/ :00:12]
30 Mohr's Circle Usage in Plane Strain A set of six Mohr's Circles representing most strain state possibilities are presented on the examples page. Also, principal directions can be computed by the principal strain calculator. Rotation Angle on Mohr's Circle Note that the coordinate rotation angle θ p is defined positive when starting at the XY coordinates and proceeding to the X p Y p coordinates. In contrast, on the Mohr's Circle θ p is defined positive starting on the principal strain line (i.e. the εaxis) and proceeding to the XY strain line (i.e. line L xy ). The angle θ p has the opposite sense between the two figures, because on one it starts on the XY coordinates, and on the other it starts on the principal coordinates. Some books avoid the sign difference between θ p on Mohr's Circle and θ p on the stress element by locating (ε x, ε xy ) instead of (ε x, ε xy ) on Mohr's Circle. This will switch the polarity of θ p on the circle. Whatever method you choose, the bottom line is that an opposite sign is needed either in the interpretation or in the plotting to make Mohr's Circle physically meaningful. Strain Transform by Mohr's Circle (2 of 4) [12/13/ :00:12]
31 Mohr's Circle Usage in Plane Strain Mohr's Circle can be used to transform strains from one coordinate set to another, similar that that described on the plane strain page. Suppose that the normal and shear strains, ε x, ε y, and ε xy, are obtained at a point O in the body, expressed with respect to the coordinates XY. We wish to find the strains expressed in the new coordinate set X'Y', rotated an angle θ from XY, as shown below: To do this we proceed as follows: Draw Mohr's circle for the given strain state (ε x, ε y, and ε xy ; shown below). Draw the line L xy across the circle from (ε x, ε xy ) to (ε y, ε xy ). Rotate the line L xy by 2*θ (twice as much as the angle between XY and X'Y') and in the opposite direction of θ. The strains in the new coordinates (ε x', ε y', and ε x'y' ) are then read off the circle. (3 of 4) [12/13/ :00:12]
32 Mohr's Circle Usage in Plane Strain Strain transforms can be performed using efunda's strain transform calculator. (4 of 4) [12/13/ :00:12]
33 Examples of Mohr's Circles in Plane Strain Examples of Mohr's Circles in Plane Strain Case 1: ε xy > 0 and ε x > ε y The principal axes are counterclockwise to the current axes (because ε xy > 0) and no more than 45º away (because ε x > ε y ). Case 2: ε xy < 0 and ε x > ε y The principal axes are clockwise to the current axes (because ε xy < 0) and no more than 45º away (because ε x > ε y ). Case 3: ε xy > 0 and ε x < ε y (1 of 3) [12/13/ :00:14]
34 Examples of Mohr's Circles in Plane Strain The principal axes are counterclockwise to the current axes (because ε xy > 0) and between 45º and 90º away (because ε x < ε y ). Case 4: ε xy < 0 and ε x < ε y The principal axes are clockwise to the current axes (because ε xy < 0) and between 45º and 90º away (because ε x < ε y ). Case 5: ε xy = 0 and ε x > ε y (2 of 3) [12/13/ :00:14]
35 Examples of Mohr's Circles in Plane Strain The principal axes are aligned with the current axes (because ε x > ε y and ε xy = 0). Case 6: ε xy = 0 and ε x < ε y The principal axes are exactly 90 from the current axes (because ε x < ε y and ε xy = 0). (3 of 3) [12/13/ :00:14]
36 Mechanics of Materials: Hooke's Law Mechanics of Materials: Hooke's Law Onedimensional Hooke's Law Robert Hooke, who in 1676 stated, The power (sic.) of any springy body is in the same proportion with the extension. announced the birth of elasticity. Hooke's statement expressed mathematically is, where F is the applied force (and not the power, as Hooke mistakenly suggested), u is the deformation of the elastic body subjected to the force F, and k is the spring constant (i.e. the ratio of previous two parameters). Generalized Hooke's Law (Anisotropic Form) Cauchy generalized Hooke's law to three dimensional elastic bodies and stated that the 6 components of stress are linearly related to the 6 components of strain. The stressstrain relationship written in matrix form, where the 6 components of stress and strain are organized into column vectors, is,, ε = S σ or,, σ = C ε where C is the stiffness matrix, S is the compliance matrix, and S = C (1 of 2) [12/13/ :00:15]
37 Mechanics of Materials: Hooke's Law In general, stressstrain relationships such as these are known as constitutive relations. In general, there are 36 stiffness matrix components. However, it can be shown that conservative materials possess a strain energy density function and as a result, the stiffness and compliance matrices are symmetric. Therefore, only 21 stiffness components are actually independent in Hooke's law. The vast majority of engineering materials are conservative. Please note that the stiffness matrix is traditionally represented by the symbol C, while S is reserved for the compliance matrix. This convention may seem backwards, but perception is not always reality. For instance, Americans hardly ever use their feet to play (American) football. (2 of 2) [12/13/ :00:15]
38 Hooke's Law for Orthotropic Materials Hooke's Law for Orthotropic Materials Orthotropic Definition Some engineering materials, including certain piezoelectric materials (e.g. Rochelle salt) and 2ply fiberreinforced composites, are orthotropic. By definition, an orthotropic material has at least 2 orthogonal planes of symmetry, where material properties are independent of direction within each plane. Such materials require 9 independent variables (i.e. elastic constants) in their constitutive matrices. In contrast, a material without any planes of symmetry is fully anisotropic and requires 21 elastic constants, whereas a material with an infinite number of symmetry planes (i.e. every plane is a plane of symmetry) is isotropic, and requires only 2 elastic constants. Hooke's Law in Compliance Form By convention, the 9 elastic constants in orthotropic constitutive equations are comprised of 3 Young's modulii E x, E y, E z, the 3 Poisson's ratios ν yz, ν zx, ν xy, and the 3 shear modulii G yz, G zx, G xy. The compliance matrix takes the form, where. (1 of 3) [12/13/ :00:16]
39 Hooke's Law for Orthotropic Materials Note that, in orthotropic materials, there is no interaction between the normal stresses σ x, σ y, σ z and the shear strains ε yz, ε zx, ε xy The factor 2 multiplying the shear modulii in the compliance matrix results from the difference between shear strain and engineering shear strain, where, etc. Hooke's Law in Stiffness Form The stiffness matrix for orthotropic materials, found from the inverse of the compliance matrix, is given by, where, The fact that the stiffness matrix is symmetric requires that the following statements hold, The factor of 2 multiplying the shear modulii in the stiffness matrix results from the difference between shear strain and engineering shear strain, where, etc. (2 of 3) [12/13/ :00:16]
40 Hooke's Law for Orthotropic Materials (3 of 3) [12/13/ :00:16]
41 Hooke's Law for Transversely Isotropic Materials Hooke's Law for Transversely Isotropic Materials Transverse Isotropic Definition A special class of orthotropic materials are those that have the same properties in one plane (e.g. the xy plane) and different properties in the direction normal to this plane (e.g. the zaxis). Such materials are called transverse isotropic, and they are described by 5 independent elastic constants, instead of 9 for fully orthotropic. Examples of transversely isotropic materials include some piezoelectric materials (e.g. PZT4, barium titanate) and fiberreinforced composites where all fibers are in parallel. Hooke's Law in Compliance Form By convention, the 5 elastic constants in transverse isotropic constitutive equations are the Young's modulus and poisson ratio in the xy symmetry plane, E p and ν p, the Young's modulus and poisson ratio in the zdirection, E pz and ν pz, and the shear modulus in the zdirection G zp. The compliance matrix takes the form, where. (1 of 3) [12/13/ :00:17]
42 Hooke's Law for Transversely Isotropic Materials The factor 2 multiplying the shear modulii in the compliance matrix results from the difference between shear strain and engineering shear strain, where, etc. Hooke's Law in Stiffness Form The stiffness matrix for transverse isotropic materials, found from the inverse of the compliance matrix, is given by, where, The fact that the stiffness matrix is symmetric requires that the following statements hold, The factor of 2 multiplying the shear modulii in the stiffness matrix results from the difference (2 of 3) [12/13/ :00:17]
43 Hooke's Law for Transversely Isotropic Materials between shear strain and engineering shear strain, where, etc. (3 of 3) [12/13/ :00:17]
44 Hooke's Law for Isotropic Materials Hooke's Law for Isotropic Materials Isotropic Definition Most metallic alloys and thermoset polymers are considered isotropic, where by definition the material properties are independent of direction. Such materials have only 2 independent variables (i.e. elastic constants) in their stiffness and compliance matrices, as opposed to the 21 elastic constants in the general anisotropic case. The two elastic constants are usually expressed as the Young's modulus E and the Poisson's ratio ν. However, the alternative elastic constants K (bulk modulus) and/or G (shear modulus) can also be used. For isotropic materials, G and K can be found from E and ν by a set of equations, and viceversa. Hooke's Law in Compliance Form Hooke's law for isotropic materials in compliance matrix form is given by, Hooke's Law in Stiffness Form The stiffness matrix is equal to the inverse of the compliance matrix, and is given by, Visit the elastic constant calculator to see the interplay amongst the 4 elastic constants (E, ν, G, K). [12/13/ :00:18]
45 Hooke's Law for Plane Stress Hooke's Law for Plane Stress Hooke's Law for Plane Stress For the simplification of plane stress, where the stresses in the z direction are considered to be negligible,, the stressstrain compliance relationship for an isotropic material becomes, The three zero'd stress entries in the stress vector indicate that we can ignore their associated columns in the compliance matrix (i.e. columns 3, 4, and 5). If we also ignore the rows associated with the strain components with zsubscripts, the compliance matrix reduces to a simple 3x3 matrix, The stiffness matrix for plane stress is found by inverting the plane stress compliance matrix, and is given by, Note that the stiffness matrix for plane stress is NOT found by removing columns and rows from the general isotropic stiffness matrix. Plane Stress Hooke's Law via Engineering Strain (1 of 2) [12/13/ :00:20]
46 Hooke's Law for Plane Stress Some reference books incorporate the shear modulus G and the engineering shear strain γ xy, related to the shear strain ε xy via, The stressstrain compliance matrix using G and γ xy are, The stiffness matrix is, The shear modulus G is related to E and ν via, (2 of 2) [12/13/ :00:20]
47 Hooke's Law for Plane Strain Hooke's Law for Plane Strain Hooke's Law for Plane Strain For the case of plane strain, where the strains in the z direction are considered to be negligible,, the stressstrain stiffness relationship for an isotropic material becomes, The three zero'd strain entries in the strain vector indicate that we can ignore their associated columns in the stiffness matrix (i.e. columns 3, 4, and 5). If we also ignore the rows associated with the stress components with zsubscripts, the stiffness matrix reduces to a simple 3x3 matrix, The compliance matrix for plane stress is found by inverting the plane stress stiffness matrix, and is given by, Note that the compliance matrix for plane stress is NOT found by removing columns and rows from the general isotropic compliance matrix. Plane Strain Hooke's Law via Engineering Strain (1 of 2) [12/13/ :00:21]
48 Hooke's Law for Plane Strain The stressstrain stiffness matrix expressed using the shear modulus G and the engineering shear strain is, The compliance matrix is, The shear modulus G is related to E and ν via, (2 of 2) [12/13/ :00:21]
49 Finding Young's Modulus and Poisson's Ratio Finding Young's Modulus and Poisson's Ratio Youngs Modulus from Uniaxial Tension When a specimen made from an isotropic material is subjected to uniaxial tension, say in the x direction, σ xx is the only nonzero stress. The strains in the specimen are obtained by, The modulus of elasticity in tension, also known as Young's modulus E, is the ratio of stress to strain on the loading plane along the loading direction, Common sense (and the 2nd Law of Thermodynamics) indicates that a material under uniaxial tension must elongate in length. Therefore the Young's modulus E is required to be nonnegative for all materials, E > 0 Poisson's Ratio from Uniaxial Tension A rodlike specimen subjected to uniaxial tension will exhibit some shrinkage in the lateral direction for most materials. The ratio of lateral strain and axial strain is defined as Poisson's ratio ν, The Poisson ratio for most metals falls between 0.25 to Rubber has a Poisson ratio close to 0.5 and is therefore almost incompressible. Theoretical materials with a Poisson ratio of exactly 0.5 are truly incompressible, since the sum of all their strains leads to a zero volume change. Cork, on the other hand, has a Poisson ratio close to zero. This makes cork function well as a bottle stopper, since an axiallyloaded cork will not swell laterally to resist bottle insertion. The Poisson's ratio is bounded by two theoretical limits: it must be greater than 1, and less than or equal to 0.5, (1 of 2) [12/13/ :00:22]
50 Finding Young's Modulus and Poisson's Ratio The proof for this stems from the fact that E, G, and K are all positive and mutually dependent. However, it is rare to encounter engineering materials with negative Poisson ratios. Most materials will fall in the range, (2 of 2) [12/13/ :00:22]
51 Finding the Shear Modulus and the Bulk Modulus Finding the Shear Modulus and the Bulk Modulus Shear Modulus from Pure Shear When a specimen made from an isotropic material is subjected to pure shear, for instance, a cylindrical bar under torsion in the xy sense, σ xy is the only nonzero stress. The strains in the specimen are obtained by, The shear modulus G, is defined as the ratio of shear stress to engineering shear strain on the loading plane, where. The shear modulus G is also known as the rigidity modulus, and is equivalent to the 2nd Lamé constant µ mentioned in books on continuum theory. Common sense and the 2nd Law of Thermodynamics require that a positive shear stress leads to a positive shear strain. Therefore, the shear modulus G is required to be nonnegative for all materials, G > 0 Since both G and the elastic modulus E are required to be positive, the quantity in the denominator of G must also be positive. This requirement places a lower bound restriction on the range for Poisson's ratio, ν > 1 Bulk Modulus from Hydrostatic Pressure (1 of 3) [12/13/ :00:24]
52 Finding the Shear Modulus and the Bulk Modulus When an isotropic material specimen is subjected to hydrostatic pressure σ, all shear stress will be zero and the normal stress will be uniform,. The strains in the specimen are given by, In response to the hydrostatic load, the specimen will change its volume. Its resistance to do so is quantified as the bulk modulus K, also known as the modulus of compression. Technically, K is defined as the ratio of hydrostatic pressure to the relative volume change (which is related to the direct strains), Common sense and the 2nd Law of Thermodynamics require that a positive hydrostatic load leads to a positive volume change. Therefore, the bulk modulus K is required to be nonnegative for all materials, K > 0 Since both K and the elastic modulus E are required to be positive, the following requirement is placed on the upper bound of Poisson's ratio by the denominator of K, ν < 1/2 Relation Between Relative Volume Change and Strain (2 of 3) [12/13/ :00:24]
53 Finding the Shear Modulus and the Bulk Modulus For simplicity, consider a rectangular block of material with dimensions a 0, b 0, and c 0. Its volume V 0 is given by, When the block is loaded by stress, its volume will change since each dimension now includes a direct strain measure. To calculate the volume when loaded V f, we multiply the new dimensions of the block, Products of strain measures will be much smaller than individual strain measures when the overall strain in the block is small (i.e. linear strain theory). Therefore, we were able to drop the strain products in the equation above. The relative change in volume is found by dividing the volume difference by the initial volume, Hence, the relative volume change (for small strains) is equal to the sum of the 3 direct strains. (3 of 3) [12/13/ :00:24]
54 Failure Criteria Failure Criteria StressBased Criteria The purpose of failure criteria is to predict or estimate the failure/yield of machine parts and structural members. A considerable number of theories have been proposed. However, only the most common and welltested theories applicable to isotropic materials are discussed here. These theories, dependent on the nature of the material in question (i.e. brittle or ductile), are listed in the following table: Material Type Ductile Brittle Failure Theories Maximum shear stress criterion, von Mises criterion Maximum normal stress criterion, Mohr's theory All four criteria are presented in terms of principal stresses. Therefore, all stresses should be transformed to the principal stresses before applying these failure criteria. Note: 1. Whether a material is brittle or ductile could be a subjective guess, and often depends on temperature, strain levels, and other environmental conditions. However, a 5% elongation criterion at break is a reasonable dividing line. Materials with a larger elongation can be considered ductile and those with a lower value brittle. Another distinction is a brittle material's compression strength is usually significantly larger than its tensile strength. 2. All popular failure criteria rely on only a handful of basic tests (such as uniaxial tensile and/or compression strength), even though most machine parts and structural members are typically subjected to multiaxial loading. This disparity is usually driven by cost, since complete multiaxial failure testing requires extensive, complicated, and expensive tests. Non StressBased Criteria (1 of 2) [12/13/ :00:25]
55 Failure Criteria The success of all machine parts and structural members are not necessarily determined by their strength. Whether a part succeeds or fails may depend on other factors, such as stiffness, vibrational characteristics, fatigue resistance, and/or creep resistance. For example, the automobile industry has endeavored many years to increase the rigidity of passenger cages and install additional safety equipment. The bicycle industry continues to decrease the weight and increase the stiffness of bicycles to enhance their performance. In civil engineering, a patio deck only needs to be strong enough to carry the weight of several people. However, a design based on the "strong enough" precept will often result a bouncy deck that most people will find objectionable. Rather, the stiffness of the deck determines the success of the design. Many factors, in addition to stress, may contribute to the design requirements of a part. Together, these requirements are intended to increase the sense of security, safety, and quality of service of the part. (2 of 2) [12/13/ :00:25]
56 Failure Criteria for Ductile Materials Failure Criteria for Ductile Materials Maximum Shear Stress Criterion The maximum shear stress criterion, also known as Tresca's or Guest's criterion, is often used to predict the yielding of ductile materials. Yield in ductile materials is usually caused by the slippage of crystal planes along the maximum shear stress surface. Therefore, a given point in the body is considered safe as long as the maximum shear stress at that point is under the yield shear stress σ y obtained from a uniaxial tensile test. With respect to 2D stress, the maximum shear stress is related to the difference in the two principal stresses (see Mohr's Circle). Therefore, the criterion requires the principal stress difference, along with the principal stresses themselves, to be less than the yield shear stress, Graphically, the maximum shear stress criterion requires that the two principal stresses be within the green zone indicated below, Von Mises Criterion (1 of 2) [12/13/ :00:26]
57 Failure Criteria for Ductile Materials The von Mises Criterion (1913), also known as the maximum distortion energy criterion, octahedral shear stress theory, or MaxwellHuberHenckyvon Mises theory, is often used to estimate the yield of ductile materials. The von Mises criterion states that failure occurs when the energy of distortion reaches the same energy for yield/failure in uniaxial tension. Mathematically, this is expressed as, In the cases of plane stress, σ 3 = 0. The von Mises criterion reduces to, This equation represents a principal stress ellipse as illustrated in the following figure, Also shown on the figure is the maximum shear stress criterion (dashed line). This theory is more conservative than the von Mises criterion since it lies inside the von Mises ellipse. In addition to bounding the principal stresses to prevent ductile failure, the von Mises criterion also gives a reasonable estimation of fatigue failure, especially in cases of repeated tensile and tensileshear loading. (2 of 2) [12/13/ :00:26]
58 Failure Criteria for Brittle Materials Failure Criteria for Brittle Materials Maximum Normal Stress Criterion The maximum stress criterion, also known as the normal stress, Coulomb, or Rankine criterion, is often used to predict the failure of brittle materials. The maximum stress criterion states that failure occurs when the maximum (normal) principal stress reaches either the uniaxial tension strength σ t, or the uniaxial compression strength σ c, σ c < {σ 1, σ 2 } < σ t where σ 1 and σ 2 are the principal stresses for 2D stress. Graphically, the maximum stress criterion requires that the two principal stresses lie within the green zone depicted below, Mohr's Theory (1 of 3) [12/13/ :00:27]
59 Failure Criteria for Brittle Materials The Mohr Theory of Failure, also known as the CoulombMohr criterion or internalfriction theory, is based on the famous Mohr's Circle. Mohr's theory is often used in predicting the failure of brittle materials, and is applied to cases of 2D stress. Mohr's theory suggests that failure occurs when Mohr's Circle at a point in the body exceeds the envelope created by the two Mohr's circles for uniaxial tensile strength and uniaxial compression strength. This envelope is shown in the figure below, The left circle is for uniaxial compression at the limiting compression stress σ c of the material. Likewise, the right circle is for uniaxial tension at the limiting tension stress σ t. The middle Mohr's Circle on the figure (dashdotdash line) represents the maximum allowable stress for an intermediate stress state. All intermediate stress states fall into one of the four categories in the following table. Each case defines the maximum allowable values for the two principal stresses to avoid failure. Case Principal Stresses Criterion requirements 1 Both in tension σ 1 > 0, σ 2 > 0 σ 1 < σ t, σ 2 < σ t 2 Both in compression σ 1 < 0, σ 2 < 0 σ 1 > σ c, σ 2 > σ c 3 σ 1 in tension, σ 2 in compression σ 1 > 0, σ 2 < 0 4 σ 1 in compression, σ 2 in tension σ 1 < 0, σ 2 > 0 (2 of 3) [12/13/ :00:27]
60 Failure Criteria for Brittle Materials Graphically, Mohr's theory requires that the two principal stresses lie within the green zone depicted below, Also shown on the figure is the maximum stress criterion (dashed line). This theory is less conservative than Mohr's theory since it lies outside Mohr's boundary. (3 of 3) [12/13/ :00:27]
61 Techniques for Failure Prevention and Diagnosis Techniques for Failure Prevention and Diagnosis There exist a set of basic techniques for preventing failure in the design stage, and for diagnosing failure in manufacturing and later stages. In the Design Stage It is quite commonplace today for design engineers to verify design stresses with finite element (FEA) packages. This is fine and good when FEA is applied appropriately. However, the popularity of finite element analysis can condition engineers to look just for red spots in simulation output, without really understanding the essence or funda at play. By following basic rules of thumb, such danger points can often be anticipated and avoided without total reliance on computer simulation. Loading Points Stress Concentrations Safety Factors Maximum stresses are often located at loading points, supports, joints, or maximum deflection points. Stress concentrations are usually located near corners, holes, crack tips, boundaries, between layers, and where crosssection areas change rapidly. Sound design avoids rapid changes in material or geometrical properties. For example, when a large hole is removed from a structure, a reinforcement composed of generally no less than the material removed should be added around the opening. The addition of safety factors to designs allow engineers to reduce sensitivity to manufacturing defects and to compensate for stress prediction limitations. In PostManufacturing Stages Despite the best efforts of design and manufacturing engineers, unanticipated failure may occur in parts after design and manufacturing. In order for projects to succeed, these failures must be diagnosed and resolved quickly and effectively. Often, the failure is caused by a singular factor, rather than an involved collection of factors. Such failures may be caught early in initial quality assurance testing, or later after the part is delivered to the customer. (1 of 2) [12/13/ :00:28]
62 Techniques for Failure Prevention and Diagnosis Induced Stress Concentrations Damage and Exposure Fatigue and Creep Stress concentrations may be induced by inadequate manufacturing processes. For example, initial surface imperfections can result from sloppy machining processes. Manufacturing defects such as size mismatches and improper fastener application can lead to residual stresses and even cracks, both strong stress concentrations. Damages during service life can lead a part to failure. Damages such as cracks, debonding, and delamination can result from unanticipated resonant vibrations and impacts that exceed the design loads. Reduction in strength can result from exposure to UV lights and chemical corrosion. Fatigue or creep can lead a part to failure. For example, unanticipated fatigue can result from repeated mechanical or thermal loading. (2 of 2) [12/13/ :00:28]
63 Nedstat Basic Wat gebeurt er... Statistieken MyNedstat Service Catalogus Hier en nu Wanneer Waarvandaan Hoe Waarmee Home Page Dr.ir. S.A. Miedema  (Software) 13 december :01 Samengevat Meet sinds... 1 mei 1999 Totaal aantal pageviews tot nu toe 8058 Drukste dag tot nu toe 27 september 2001 Pageviews 67 Prognose voor vandaag Gemiddeld komt 41 procent van het dagelijkse bezoek vóór 13:01. Op grond van het bezoekersaantal van 10 van vandaag tot nu toe kan uw site vandaag op 24 pageviews (+/ 4) uitkomen. Laatste 10 bezoekers december 02:43 Nottingham, Verenigd Koninkrijk (djanogly.notts.) december 03:05 Nottingham, Verenigd Koninkrijk (djanogly.notts.) december 07:11 ALLTEL, Verenigde Staten december 08:25 TU Delft, Delft, Nederland december 08:27 TU Delft, Delft, Nederland december 08:32 TU Delft, Delft, Nederland december 10:09 TU Delft, Delft, Nederland december 10:58 TU Delft, Delft, Nederland december 12:26 Chinanet, China december 13:00 TU Delft, Delft, Nederland Pageviews per dag (1 of 3) [12/13/ :00:38]
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More information1 Stress and Strain. Introduction
1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationGATE SOLUTIONS E N G I N E E R I N G
GATE SOLUTIONS C I V I L E N G I N E E R I N G From (1987018) Office : F16, (Lower Basement), Katwaria Sarai, New Delhi110016 Phone : 01165064 Mobile : 81309090, 9711853908 Email: info@iesmasterpublications.com,
More informationA short review of continuum mechanics
A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 12.510 Introduction to Seismology Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Stress and Strain
More informationVYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA
VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Overview Milestones in continuum mechanics Concepts of modulus and stiffness. Stressstrain relations Elasticity Surface and body
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationPrincipal Stresses, Yielding Criteria, wall structures
Principal Stresses, Yielding Criteria, St i thi Stresses in thin wall structures Introduction The most general state of stress at a point may be represented by 6 components, x, y, z τ xy, τ yz, τ zx normal
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationUse Hooke s Law (as it applies in the uniaxial direction),
0.6 STRSSSTRAIN RLATIONSHIP Use the principle of superposition Use Poisson s ratio, v lateral longitudinal Use Hooke s Law (as it applies in the uniaxial direction), x x v y z, y y vx z, z z vx y Copyright
More informationChapter 6: Plastic Theory
OHP Mechanical Properties of Materials Chapter 6: Plastic Theory Prof. Wenjea J. Tseng 曾文甲 Department of Materials Engineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W. F.
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationTable of Contents. Preface...xvii. Part 1. Level
Preface...xvii Part 1. Level 1... 1 Chapter 1. The Basics of Linear Elastic Behavior... 3 1.1. Cohesion forces... 4 1.2. The notion of stress... 6 1.2.1. Definition... 6 1.2.2. Graphical representation...
More informationPlasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur
Plasticity R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 9 Table of Contents 1. Plasticity:... 3 1.1 Plastic Deformation,
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationNDT&E Methods: UT. VJ Technologies CAVITY INSPECTION. Nondestructive Testing & Evaluation TPU Lecture Course 2015/16.
CAVITY INSPECTION NDT&E Methods: UT VJ Technologies NDT&E Methods: UT 6. NDT&E: Introduction to Methods 6.1. Ultrasonic Testing: Basics of ElastoDynamics 6.2. Principles of Measurement 6.3. The PulseEcho
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationStatic Failure (pg 206)
Static Failure (pg 06) All material followed Hookeʹs law which states that strain is proportional to stress applied, until it exceed the proportional limits. It will reach and exceed the elastic limit
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationMECH 401 Mechanical Design Applications
MECH 401 Mechanical Design Applications Dr. M. O Malley Master Notes Spring 008 Dr. D. M. McStravick Rice University Updates HW 1 due Thursday (11708) Last time Introduction Units Reliability engineering
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More information202 Index. failure, 26 field equation, 122 force, 1
Index acceleration, 12, 161 admissible function, 155 admissible stress, 32 Airy's stress function, 122, 124 d'alembert's principle, 165, 167, 177 amplitude, 171 analogy, 76 anisotropic material, 20 aperiodic
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationEquilibrium of Deformable Body
Equilibrium of Deformable Body Review Static Equilibrium If a body is in static equilibrium under the action applied external forces, the Newton s Second Law provides us six scalar equations of equilibrium
More informationMAE 322 Machine Design Lecture 2. Dr. Hodge Jenkins Mercer University
MAE 322 Machine Design Lecture 2 Dr. Hodge Jenkins Mercer University Statics Load Failure Theories to Understand Maximum Normal Stress (MNS) Maximum Shear Stress (MSS) Distortion Energy (DE) CoulombMohr
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More information3.22 Mechanical Properties of Materials Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 3.22 Mechanical Properties of Materials Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Quiz #1 Example
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationMacroscopic theory Rock as 'elastic continuum'
Elasticity and Seismic Waves Macroscopic theory Rock as 'elastic continuum' Elastic body is deformed in response to stress Two types of deformation: Change in volume and shape Equations of motion Wave
More information7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment
7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that
More informationTensor Transformations and the Maximum Shear Stress. (Draft 1, 1/28/07)
Tensor Transformations and the Maximum Shear Stress (Draft 1, 1/28/07) Introduction The order of a tensor is the number of subscripts it has. For each subscript it is multiplied by a direction cosine array
More informationANALYSIS OF STRAINS CONCEPT OF STRAIN
ANALYSIS OF STRAINS CONCEPT OF STRAIN Concept of strain : if a bar is subjected to a direct load, and hence a stress the bar will change in length. If the bar has an original length L and changes by an
More informationCHAPTER 2 Failure/Fracture Criterion
(11) CHAPTER 2 Failure/Fracture Criterion (12) Failure (Yield) Criteria for Ductile Materials under Plane Stress Designer engineer: 1 Analysis of loading (for simple geometry using what you learn here
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More informationMECHANICS OF MATERIALS
Third CHTR Stress MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University and Strain xial oading Contents Stress & Strain: xial oading Normal
More informationStrength of Materials Prof. S.K.Bhattacharya Dept. of Civil Engineering, I.I.T., Kharagpur Lecture No.26 Stresses in BeamsI
Strength of Materials Prof. S.K.Bhattacharya Dept. of Civil Engineering, I.I.T., Kharagpur Lecture No.26 Stresses in BeamsI Welcome to the first lesson of the 6th module which is on Stresses in Beams
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationExercise: concepts from chapter 5
Reading: Fundamentals of Structural Geology, Ch 5 1) Study the oöids depicted in Figure 1a and 1b. Figure 1a Figure 1b Figure 1. Nearly undeformed (1a) and significantly deformed (1b) oöids with spherulitic
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More information2.1 Background of Piping Stresses
2 Research Review One of the major additions to Tmin was the inclusion of analysis of a 2Dimensional vertical piping span. The original plan from Dupont was to include several types of 2D and 3D vertical
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure
More informationLecture M1 Slender (one dimensional) Structures Reading: Crandall, Dahl and Lardner 3.1, 7.2
Lecture M1 Slender (one dimensional) Structures Reading: Crandall, Dahl and Lardner 3.1, 7.2 This semester we are going to utilize the principles we learnt last semester (i.e the 3 great principles and
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More information20. Rheology & Linear Elasticity
I Main Topics A Rheology: Macroscopic deformation behavior B Linear elasticity for homogeneous isotropic materials 10/29/18 GG303 1 Viscous (fluid) Behavior http://manoa.hawaii.edu/graduate/content/slidelava
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationERM  Elasticity and Strength of Materials
Coordinating unit: Teaching unit: Academic year: Degree: ECTS credits: 2018 205  ESEIAAT  Terrassa School of Industrial, Aerospace and Audiovisual Engineering 712  EM  Department of Mechanical Engineering
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationStrain Transformation equations
Strain Transformation equations R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Stress transformation
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationStructural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationComb resonator design (2)
Lecture 6: Comb resonator design () Intro Intro. to Mechanics of Materials School of Electrical l Engineering i and Computer Science, Seoul National University Nano/Micro Systems & Controls Laboratory
More informationModule 5: Theories of Failure
Module 5: Theories of Failure Objectives: The objectives/outcomes of this lecture on Theories of Failure is to enable students for 1. Recognize loading on Structural Members/Machine elements and allowable
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationStress and Strain ( , 3.14) MAE 316 Strength of Mechanical Components NC State University Department of Mechanical & Aerospace Engineering
(3.83.1, 3.14) MAE 316 Strength of Mechanical Components NC State Universit Department of Mechanical & Aerospace Engineering 1 Introduction MAE 316 is a continuation of MAE 314 (solid mechanics) Review
More informationStrain Measurements. Isaac Choutapalli
Note that for axial elongation (Eaxiai > 0), Erransverse (from Equation C.6), and therefore Strain Measurements Isaac Choutapalli Department of Mechanical Engineering The University of Texas  Pan American
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationRock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth
Rock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth References: Turcotte and Schubert, Geodynamics, Sections 2.1,2.4, 2.7, 3.13.8, 6.1, 6.2, 6.8, 7.17.4. Jaeger and Cook, Fundamentals of
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationTheory of Plasticity. Lecture Notes
Theory of Plasticity Lecture Notes Spring 2012 Contents I Theory of Plasticity 1 1 Mechanical Theory of Plasticity 2 1.1 Field Equations for A Mechanical Theory.................... 2 1.1.1 Straindisplacement
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationCHAPTER 4 Stress Transformation
CHAPTER 4 Stress Transformation ANALYSIS OF STRESS For this topic, the stresses to be considered are not on the perpendicular and parallel planes only but also on other inclined planes. A P a a b b P z
More informationReview Lecture. AE1108II: Aerospace Mechanics of Materials. Dr. Calvin Rans Dr. Sofia Teixeira De Freitas
Review Lecture AE1108II: Aerospace Mechanics of Materials Dr. Calvin Rans Dr. Sofia Teixeira De Freitas Aerospace Structures & Materials Faculty of Aerospace Engineering Analysis of an Engineering System
More informationChapter 1. Continuum mechanics review. 1.1 Definitions and nomenclature
Chapter 1 Continuum mechanics review We will assume some familiarity with continuum mechanics as discussed in the context of an introductory geodynamics course; a good reference for such problems is Turcotte
More informationStress transformation and Mohr s circle for stresses
Stress transformation and Mohr s circle for stresses 1.1 General State of stress Consider a certain body, subjected to external force. The force F is acting on the surface over an area da of the surface.
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationELASTICITY (MDM 10203)
ELASTICITY () Lecture Module 3: Fundamental Stress and Strain University Tun Hussein Onn Malaysia Normal Stress inconstant stress distribution σ= dp da P = da A dimensional Area of σ and A σ A 3 dimensional
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More information